Characterization of Microstructure and Mechanical ... of Microstructure and Mechanical Properties...
Embed Size (px)
Transcript of Characterization of Microstructure and Mechanical ... of Microstructure and Mechanical Properties...
Metals 2015, 5, 1704-1716; doi:10.3390/met5031704
metals ISSN 2075-4701
Characterization of Microstructure and Mechanical Properties
of Resistance Spot Welded DP600 Steel
Ali Ramazani 1,*, Krishnendu Mukherjee 2, Aydemir Abdurakhmanov 3, Mahmoud Abbasi 4
and Ulrich Prahl 2
1 Department of Chemical Engineering, University of Michigan, Ann Arbor, MI 48109, USA 2 Department of Ferrous Metallurgy, RWTH Aachen University, Aachen 52072, Germany;
E-Mails: email@example.com (K.M.);
firstname.lastname@example.org (U.P.) 3 Welding and Joining Institute, RWTH Aachen University, Aachen 52072, Germany;
E-Mail: email@example.com 4 Faculty of Engineering, University of Kashan, Kashan-8731751167, Iran;
* Author to whom correspondence should be addressed; E-Mail: firstname.lastname@example.org;
Tel.: +1-734-353-3569; Fax: +1-734-763-0459.
Academic Editor: Hugo F. Lopez
Received: 9 July 2015 / Accepted: 13 September 2015 / Published: 17 September 2015
Abstract: Resistance spot welding (RSW) as a predominant welding technique used for
joining steels in automotive applications needs to be studied carefully in order to improve
the mechanical properties of the spot welds. The objectives of the present work are to
characterize the resistance spot weldment of DP600 sheet steels. The mechanical properties
of the welded joints were evaluated using tensile-shear and cross-tensile tests. The
time-temperature evolution during the welding cycle was measured. The microstructures
observed in different sites of the welds were correlated to thermal history recorded by
thermocouples in the corresponding areas. It was found that cracks initiated in the
periphery region of weld nuggets with a martensitic microstructure and a pull-out failure
mode was observed. It was also concluded that tempering during RSW was the main
reason for hardness decrease in HAZ.
Metals 2015, 5 1705
Keywords: resistance spot welding; dual-phase steel; microstructure; tensile-shear test;
cross-tensile test; hardness map; fracture
The main focus of the automotive industry is to reduce the weight of car, enhance safety and
crashworthiness while the cost is low . In comparison with traditional low carbon and high
strength low alloy steels, dual phase (DP) steels provide a combination of good formability and
strength [4,5]. DP steels are attractive to automakers as they can offer safety, affordability, fuel
efficiency, and environmental responsibility . Wang et al.  studied the high strain rate behavior
of high strength DP steels. They reported that for high strain rate tests, comparable to crash situations,
the DP steels fail in ductile mode. The microstructure of DP steel consists of hard martensite particles
dispersed in a soft, ductile ferrite matrix. A well-balanced ratio between ferrite and martensite volume
fractions has been reported to be the most important factor affecting the mechanical properties of DP
steels [10,11]. The other factors affecting the mechanical behavior includes: the morphology of the
martensite islands, carbon content in the martensite, and the deformation condition of ferrite, i.e.,
dislocation density [12,13].
Welding is the most important joining technique in the automotive industry, and its condition plays
a prominent role in determining the final mechanical properties of the joints. Local heat input from the
welding heat source induces a large temperature gradient on the workpiece and it may destroy the
microstructure and hence the mechanical properties of steels . This holds in particular for DP steels
which contain a specific ferritic-martensitic microstructure [15,16]. It is, therefore, important to
characterize the microstructure evolution during welding and its influence on the final mechanical
properties of DP steels.
Resistance Spot Welding (RSW) is the primary sheet metal welding process in the manufacture of
automotive assemblies . The embedded infrastructure makes RSW an economically-desirable
process. The failure modes of steel RSWs are button pull-out, partial pull-out, and interfacial fracture,
where the button pull-out is preferred as more energy is absorbed during this kind of failure .
Zhang et al.  reported that the failure mode primarily depends on the fusion zone size and failure
tends to occur under pull-out mode as fusion zone size increases. Ma et al.  reported about the
formation of shrinkage voids in fusion zone of spot-welded DP600 steel. According to them, these
voids are formed due to rich chemistry of DP steels as compared to low carbon steels.
According to the industrial standards, the minimum size of the spot welds to guarantee the pull-out
fracture follows the relation D = Kt, where D is the weld nugget diameter in mm, K is a
process-dependent constant ranging from 3 to 6, and t is the minimum sheet thickness in mm [21,22].
Pouranvari et al.  discussed a new criterion to ensure button pull-out failure for advanced high
strength steels. Khan et al.  studied the effects of alloying elements and processing techniques on
failure modes of AHSS steels RSWs. They concluded that steels with higher carbon content had higher
FZ hardness demonstrating a strong relationship between chemistry and mechanical properties.
They compared the failure characteristic of DP600 galvanized sheets RSWs with that of DP780
Metals 2015, 5 1706
galvannealed sheets. The DP600 galvanized steel failed by interfacial mode, whereas the DP780
galvannealed steel failed by button pull-out mode. Hayat et al.  have studied the effect of welding
parameters on fracture toughness of galvanized DP600 automotive steel sheets RSWs. They concluded
that the fracture toughness of RSW depends on the nugget diameter, sheet thickness, tensile rupture
force, welding time, and current. Hernandez et al.  studied the behavior of dissimilar weldment of
DP600 with other advanced high strength steels. They reported pull-out failure mode is observed when
DP600 is welded to other advanced high strength steels, compared to DP600 steel.
In the current research, the microstructure and mechanical properties of resistance spot welded
DP600 steel was analyzed. Different microstructures of various sites were analyzed according to their
thermal history during welding process. Additionally, mechanical properties of welded spots were
investigated through tensile-shear and cross-tensile tests as well as hardness testing. Fractography
analyses were conducted to reveal the fracture mode.
2. Experimental Techniques
2.1. Material Characterization
The material used in this study, supplied by ThyssenKrupp Steel AG Division Auto (Essen,
Germany), is cold rolled galvanized sheet of DP600 steel with 1.5 mm thickness. As can be seen from
the chemical composition listed in Table 1, the material is a low carbon steel, with additions of a
relatively high level of manganese, plus some Si and Cr to facilitate the formation of the dual phase
microstructure and to offer the aimed properties.
Table 1. The chemical composition of the investigated DP steel- in weight-%.
C Si Mn Cr Mo Al
0.09 0.2 1.24 0.14 0.2 0.026
The results of SEM (Figure 1) showed that the initial microstructures consisted of 85% ferrite and
15% martensite. The average ferrite grain size was 7 m.
Figure 1. SEM picture of the studied base material.
Metals 2015, 5 1707
2.2. Welding Experiment
The investigations were conducted on a C-shaped robot spot welding gun with a medium-frequency
direct-current transformer (RWTH-Aachen University, Aachen, Germany). Water-cooled electrode
caps of the G16 type according to DIN ISO 5821 were used for the welding tests, with a working
surface of 6 mm.
Welding samples were prepared from cold rolled plates. The plates were machined into specimens
of 83 45 1.5 mm3 and finally they were welded together. The values of force, current, and time
parameters used in this study are reported in Table 2. The parameter values were selected in such a
way that, the minimum nugget diameter of 4*t, where t is the sheet thickness, was obtained after
RSW and they were corresponded to welding parameters close to industrial conditions. For each sample,
metallographic examination was carried out to reveal the microstructure. Tensile-shear, cross-tensile
tests, as well as the hardness testing were applied to evaluate the mechanical properties. Three
tensile-shear tests and three cross-tensile tests were performed.
Table 2. The operation conditions for RSW.
FEI [kN] Hold-back time [ms] IS1 [kA] tS1 [ms]
3 140 7 200
The cooling rate has important influence on the formation of microstructure in the weld nugget and
HAZ. To get thermal cycles of different places, three thermocouples Type K (chromelalumel) were
fixed at different distances from the weld spot. The distances were chosen to be 2.9, 3.5, and 4.3 mm,
as shown in Figure 2. Thermocouples were situated on positions away from welding electrodes to
inhibit the damage.
Figure 2. The location of the thermocouples.